In-Vitro Comparative Study of the Effect of
Four Finishing and Polishing Tools on
Sur-face Roughness of a Microhybrid Resin
S Nemati Anarakiu1
, Z GHafari3
, Z Naser4
, T Bitaraf*5
1- Assistant professor, Restorative Dept, faculty of Dentistry,Tehran medical sciences, Islamic Azad University, Tehran, Iran.
2- Assistant professor, Restorative Dept, Dental implant research center faculty of Dentistry,Tehran medical sciences, Islamic Azad University, Tehran, Iran.
3- Dentist, Tehran, Iran
4- Dentist, Boston, Massachusetts, United States.
5- Assistant professor, Dental Implant Research Center, Dental Faculty, Tehran Medical Sciences, Islamic Azad Univer-sity, Tehran, Iran
ABSTRACT ARTICLE INFO
Received: March 2018 Accepted: April 2018 ePublished: May 2019
Assistant professor, Dental Implant Re-search Center, Dental Faculty, Tehran Medical Sciences, Islamic Azad University, Tehran, Iran , taherehbitaraf@ yahoo.com
Background and Aim: The complications of unwanted surface roughness of com-posite restorations are highly common due to the increasing use of this restorative
ma-terial. Therefore, the present study was designed to compare the effect of four finish -ing and polish-ing (F&P) tools on surface roughness of microhybrid resin composites.
Materials and Methods: This experimental study was performed on 42 samples of CLEARFIL™ AP-X microhybrid composite, which were divided into four groups of different F&P methods and one control group as follows: control (n=2), Flexi-D discs (n=10), Flexi-D + diamond polishing paste (n=10), Intensive twisted rubber polisher (n=10), and Rubber Polisher Teco (n=10). The samples were examined by
profilometry. Surface roughness (Ra) of each specimen was measured at three points,
and the mean value was considered as surface roughness. The results were analyzed by analysis of variance (ANOVA) and post hoc statistical tests.
Results:The surface roughness of composite discs in an ascending order was as fol-lows: control (0.048±0.014 µm), Flexi-D disc (0.179±0.132 µm), Intensive twist-ed rubber polisher (0.233±0.105 µm), Flexi-D disc with diamond polishing paste (0.232±0.141 µm), and Rubber Polisher Teco (0.251±0.087 µm; P=0.001). The dif-ference between the two groups of Flexi-D disc with diamond polishing paste and
Rubber Polisher Teco was not statistically significant (P=0.742). The level of surface roughness in Flexi-D samples was significantly lower than that of the other samples
Conclusion:It seems that the Flexi-D disc is the best F&P tool for microhybrid resin composites.
Keywords:Dental Polishing / Instrumentation, Composite Resin, Surface Properties, Ma-terials Testing
J Res Dentomaxillofac Sci 2019;4(2):26-31. DOI: 10.29252/jrdms.4.2.26
The surface roughness of restorative materials is one of the problems that can cause plaque and bacteria to accumulate, eventually leading to un-healthy surfaces with consequences such as dis-coloration and gingival and periodontal inflam -mation. (1-3)
Also, increased staining of composite restorations will ultimately have a significant effect on their aes -thetics. The maximum acceptable roughness is 0.2 μm for restorative materials; at this level, there will be no bacterial adhesion. Higher surface roughness will cause bacterial adhesion and plaque accumula-tion, increasing the risk of decay and
http://www.jrdms.dentaliau.ac.ir Journal of Research in dental and maxillofacial sciences 27
Finishing and polishing (F&P) techniques are used to reduce the surface roughness of restora-tive materials. Finishing (shaping or reducing re-storative materials for ideal anatomy) and polish-ing (reduction of roughness and scratches created by polishing tools on the restoration) are very important stages of restoration that affect both the aesthetics and the longevity of the final res -toration.(2,3)
The final shaping and polishing of resin com -posites can be accomplished by various means. Diamond burs, carbide burs, various types of rubber point, rubbers, and polishing pastes are among the means of polishing.(1,4-8)
Previous studies have investigated the surface roughness of microhybrid resin composites af-ter F&P with aluminum oxide disc alone or alu-minum disc with another F&P method (carbide bur, diamond bur or diamond paste).(9-16)
In these studies, when using aluminum disc (Sof-Lex) alone, the surface roughness of the mi-crohybrid composite was significantly reduced, and the addition of another method to Sof-Lex failed to improve the surface roughness.(9-16)
The effect of new F&P tools, such as Rubber Polisher Teco (silicon composite resin polishing disc), Flexi-D disc (EVE; flexible aluminum ox -ide disc for composite, gold, and amalgam pol-ishing), and Intensive twisted rubber polisher (composite polishing disc), on the surface rough-ness of composite resins has been limitedly in-vestigated.(16-21)
In the present study, the effects of four types of F&P tools, including Rubber Polisher Teco, Intensive twisted rubber polisher, Flexi-D disc, and diamond polishing paste, on the surface roughness of microhybrid resin composites were investigated in vitro.
Materials and Methods
In this in-vitro experimental study, 42 samples in four groups of 10 each and one control group of two samples were prepared. The simple rand-omization method was used for sampling. First, a polyvinyl chloride (PVC) mold with a diameter of 6 mm and a thickness of 3 mm and resistant to deformation was provided. To prepare each
specimen, the mold was placed on a glass slab on which a celluloid strip (BP, Iran) was placed. This was done to prevent the adhesion of the composite to the glass slab during the curing of the compos-ite. The CLEARFIL™ AP-X composites (Kurar-ay Noritake Dental Inc., Ok(Kurar-ayama, Japan) were then placed in layers of less than 2-mm thickness inside the mold in two steps and cured during two steps. The thickness of the first layer of the com -posite was 1 mm. For curing the last layer, the celluloid strip was placed on the mold. The glass slide was then placed on the celluloid strip, and the final pressure was applied to the specimen so that the glass slide would be in direct contact with the mold edges and the excess composite would be ejected. Specimens were cured from beyond the glass slide after visual assurance of the ab-sence of any bubbles or incomplete compaction. Overlap curing was performed for 20 seconds at each stage with the intensity of 1000 mW/cm2 (J. Morita Mfg. Corp., Kyoto, Japan) at a distance of 1 mm from the surface of the specimens.(15) The
intensity of the light-curing unit was checked at each stage using a radiometer.
The samples were then randomly divided into five identical groups. All composite specimens were finished and polished in a wet environment for 30 seconds with each tool. (15,21) The groups
were as follows:
Control group, which remained intact,Flexi-D group (EVE Ernst Vetter GmbH; Pforzheim, Ger-many): flexible aluminum oxide discs for com -posite, gold, and amalgam polishing,
Intensive twisted rubber polisher group (EVE Ernst Vetter GmbH; Pforzheim, Germany): sili-cone composite polishing discs,
Rubber polisher Teco group (EVE Ernst Vet-ter GmbH; Pforzheim, Germany): silicone com-posite polishing discs,
Diamond polishing paste group (DiaPolisher Paste, GC Europe, Leuven, Belgium): the final finishing of composite and ceramic restorations with abrasive particles of 1 to 2 microns.
Surface roughness (Ra) of each specimen was measured at three points, and the mean value was considered as the average surface rough-ness (Ra).(21) The Ra data were statistically
ana-lyzed by analysis of variance (ANOVA) and post hoc supplementary statistical tests. The samples were compared overall and then pair-wise.
Result:This study included 42 specimens: 10 in each group and two in the control group. The surface roughness (µm) of each group is presented in Table 1 and Figure 1. As shown in the table, the highest level of surface roughness was detected in the Rubber Polisher Teco group (0.251±0.087 μm), and the lowest, except for the control group, was detected in the Flexi-D (EVE) group (0.179±0.132 μm).
According to ANOVA, the lowest surface roughness in the four groups (regardless of the control group) was observed in the Flexi-D (EVE) group (0.179±0.132 µm). The difference between surface roughness in the four groups was statistically significant according to ANO -VA (P<0.001).
Table 1: Surface roughness (µm) of the samples of each studied group
Flexi-D (EVE) disc 0.179±0.132
Flexi-D (EVE) disc+ diamond polishing paste
Rubber Polisher Teco 0.251±0.087
Intensive twisted rubber polisher
Least significant difference (LSD) and Tukey’s post hoc tests were used for the comparison of the mean surface roughness between each two groups, which showed that the differences between the control group and all four Flexi-D (EVE) (P=0.01), Flexi-Flexi-D (EVE) + diamond polishing paste (P<0.001), Rubber Polisher Teco (P<0.001), and Intensive twisted rubber polisher (P<0.001) groups were statistically significant. Surface roughness was significantly higher in D (EVE) samples than in Flexi-D (EVE) + diamond polishing paste (P=0.036), Rubber Polisher Teco (P=0.016), and Intensive twisted rubber polisher (P=0.047) samples. The difference between Flexi-D (EVE) + diamond polishing paste and Rubber Polisher Teco was not statistically significant (P=0.742), but the surface roughness in Intensive twisted rub-ber polisher samples was significantly lower compared to Flexi-D (EVE) + diamond polish-ing paste and Rubber Polisher Teco samples (P<0.05).
Figure 1. Surface roughness (µm) of each sample in the studied groups
http://www.jrdms.dentaliau.ac.ir Journal of Research in dental and maxillofacial sciences 29
However, the surface roughness of microhy-brid composites after F&P by Sof-Lex with an-other F&P method ranged from 0.074 to 0.23 μm.
(16-19) In these studies, when using Sof-Lex alone,
the surface roughness of the microhybrid com-posite was significantly reduced, and the addition of another method to Sof-Lex failed to improve surface roughness. In a 2015 study by Ferriera et al, Sof-Lex alone produced surface roughness equal to 0.01 μm, while Sof-Lex together with diamond paste produced surface roughness equal to 0.1 μm.(15) A study performed by Botta et al
showed that the surface roughness after the use of Diamond flex with diamond paste was 0.074 μm while adding Diamond pro to the above composi-tion caused surface roughness to increase to 0.079 µm. (19) The results of other methods of F&P used in the present study (two groups of Rubber polisher Teco and Intensive twisted rubber polisher) are con-sistent with previous studies.(20,21)
CLEARFIL™ AP-X composite consists of Bis-GMA, TEGDMA, silanized barium glass filler, si -lanized silica filler, si-lanized colloidal silica, cam -phorquinone, accelerators, catalysts, and pigments. Filler particle size is 0.3 µm, 86% by weight and 70% by volume.
In F&P, if abrasive components are not harder than the filler inside the composite, the polisher only removes the matrix and soft parts, while the fillers remain on the surface. Therefore, unlike silicone discs, aluminum discs are capable of bet-ter polishing of CLEARFIL™ AP-X composite, which includes barium glass and silica fillers.(9) In
the present study (except for the control group due to its small sample size), the lowest surface rough-ness was related to Flexi-D disc (aluminum oxide). In previous studies on microfilled composites, Sof-Lex discs (aluminum oxide) produced the lowest surface roughness compared to other samples.(8,9)
The surface morphology of composite resins af-ter F&P is affected by various factors such as the size, hardness, and amount of filler particles.(22) In
polishing, if the filler particles are hard, bumps are created on the surface of hybrid composites while the soft matrix resin disappears. Filler particles must be close together to protect the resin matrix. The smaller the filler particles, the lower is the po -lymerization, the higher is the shrinkage and the more are mechanical problems.(22,23)
Compared to microfilled and hybrid composites,
nanofilled composites have the highest polish -ability. In previous studies, hybrid composites (Filtek Z250) showed the lowest surface smooth-ness, which can be attributed to the formation of large glass filler particles that, when compressed, leave bubbles and rough surfaces after polishing.
(22-25) Hybrid composites have larger filler parti
-cles than nanofilled and microfilled composites, which is why their surface roughness is even greater. Because of the different types of filler particles and resin, it is important to use a polish-ing system that is compatible with the resin com-posite.(11,25)
In our study and many previous studies, only surface roughness was measured, which is only one of several parameters that affect the quality of restorative surfaces in the clinical setting. Oth-er effective factors, such as the amount of pres-sure applied during polishing, the direction of the surface, the time taken during the F&P process, and the abrasives used for polishing, affect sur-face roughness.(26,27) In the present study, we tried
to prevent these confounders from affecting the results; however, some of these factors are inevi-table. Future studies with better control of these confounders are suggested.
In the present study, Flexi-D disc produced the lowest surface roughness in CLEARFIL™ AP-X light-cure composite. It can, therefore, be of good quality in clinical practice. However, since the present research has been done on flat surfaces and in a laboratory environment, its application in clinical practice depends on the position of the tooth and the polishing area; F&P on prominent surfaces, especially in the posterior teeth, can al-ter the results. Also, in this study, only surface roughness was investigated, and other aspects including composite color, aesthetics, thickness, biofilm and microorganism accumulation, re -sistance, and other characteristics need further investigation.
9. Antonson SA, Yazici AR, Kilinc E, Anton-son DE, Hardigan PC. CompariAnton-son of different finishing/polishing systems on surface rough -ness and gloss of resin composites. J Dent. 2011 Jul;39 Suppl 1:e9-17.
10. da Costa JB, Goncalves F, Ferracane JL. Comparison of two-step versus four-step com-posite finishing/polishing disc systems: evalua -tion of a new two-step composite polishing disc system. Oper Dent. 2011 Mar-Apr;36(2):205-12. 11. de Moraes RR, Gonçalves Lde S, Lancellotti AC, Consani S, Correr-Sobrinho L, Sinhoreti MA. Nanohybrid resin composites: nanofiller loaded materials or traditional microhybrid res-ins? Oper Dent. 2009 Sep-Oct;34(5):551-7. 12. Janus J, Fauxpoint G, Arntz Y, Pelletier H, Etienne O. Surface roughness and morphology of three nanocomposites after two different pol-ishing treatments by a multitechnique approach. Dent Mater. 2010 May;26(5):416-25.
13. Senawongse P, Pongprueksa P. Surface rough-ness of nanofill and nanohybrid resin composites after polishing and brushing. J Esthet Restor Dent. 2007;19(5):265-73; discussion 274-5. 14. Silikas N, Kavvadia K, Eliades G, Watts D. Surface characterization of modern resin com-posites: a multitechnique approach. Am J Dent. 2005 Apr;18(2):95-100.
15.Ferreira PM, Souto SH, Borges BC, de Assun-ção IV, da Costa GD. Impact of a novel polishing method on the surface roughness and micromor-phology of nanofilled and microhybrid compos -ite resins. Rev Port deEstomatol Med Dent Cir Maxillofac. 2015 Jan-Mar;56(1):18–24.
16. Daud A, Gray G, Lynch CD, Wilson NHF, Blum IR. A randomised controlled study on study on the use of finishing and polishing systems on different resin composites using 3D contact op-tical profilometry and scanning electron micros -copy. J Dent. 2018 Apr;71:25-30.
17. Gönülol N, Yilmaz F. The effects of finishing and polishing techniques on surface roughness and color stability of nanocomposites. J Dent. 2012 Dec;40 Suppl 2:e64-70.
18. Turssi CP, Ferracane JL, Serra MC. Abrasive wear of resin composites as related to finish -ing and polish-ing procedures. Dent Mater. 2005 Jul;21(7):641-8.
above results requires further in-vivo studies in clinical settings.
We would like to acknowledge the support of the Vice Chancellor for Research of the Faculty of Dentistry, Islamic Azad University of Medi-cal Sciences, Tehran, Iran. It should be noted that this study has been derived from thesis no. 25633.
1.Cenci MS, Venturini D, Pereira-Cenci T, Piva E, Demarco FF. The effect of polishing tech-niques and time on the surface characteristics and sealing ability of resin composite restora-tions after one-year storage. Oper Dent. 2008 Mar-Apr;33(2):169-76.
2.Oliveira ALBMd, Garcia PPNS, Santos PAd, Campos JÁDB. Surface roughness and hard-ness of a composite resin: influence of finishing and polishing and immersion methods. Mater Res. 2010;13(3):409-15.
3. Ortengren U, Wellendorf H, Karlsson S, Ruyter IE. Water sorption and solubility of den-tal composites and identification of monomers released in an aqueous environment. J Oral Re-habil. 2001 Dec;28(12):1106-15.
4. Venturini D, Cenci MS, Demarco FF, Cama-cho GB, Powers JM. Effect of polishing tech-niques and time on surface roughness, hardness and microleakage of resin composite restora-tions. Oper Dent. 2006 Jan-Feb;31(1):11-7. 5. Yap AU, Ong SB, Yap WY, Tan WS, Yeo JC. Surface texture of resin-modified glass ionomer cements: effects of finishing/polishing time. Oper Dent. 2002 Sep-Oct;27(5):462-7.
http://www.jrdms.dentaliau.ac.ir Journal of Research in dental and maxillofacial sciences 31
19. Botta AC, Duarte S Jr, Paulin Filho PI, Gheno SM, Powers JM. Surface roughness of enamel and four resin composites. Am J Dent. 2009;22(5):252-4.
20. Aytac F, Karaarslan ES, Agaccioglu M, Tastan E, Buldur M, Kuyucu E. Effects of Nov-el Finishing and Polishing Systems on Surface Roughness and Morphology of Nanocompos-ites. J Esthet Restor Dent. 2016 Jul;28(4):247-61.
21. Cazzaniga G, Ottobelli M, Ionescu AC, Paolone G, Gherlone E, Ferracane JL, et al. In vitro biofilm formation on resin-based compos -ites after different finishing and polishing proce -dures. J Dent. 2017 Dec;67:43-52.
22. Yadav RD, Raisingani D, Jindal D, Mathur R. A Comparative Analysis of Different Finish-ing and PolishFinish-ing Devices on Nanofilled, Micro -filled, and Hybrid Composite: A Scanning Elec -tron Microscopy and Profilometric Study. Int J Clin Pediatr Dent. 2016 Jul-Sep;9(3):201-208. 23. Ergücü Z, Türkün LS. Surface rough-ness of novel resin composites polished with one-step systems. Oper Dent. 2007 Mar-Apr;32(2):185-92.
24. Yalcin F, Korkmaz Y, Baseren M. The effect of two different polishing techniques on micro-leakage of new composites in Class V restora-tions. J Contemp Dent Pract. 2006;7(5):18-25. 25. Kaizer MR, de Oliveira-Ogliari A, Cenci MS, Opdam NJ, Moraes RR. Do nanofill or sub -micron composites show improved smoothness and gloss? A systematic review of in vitro stud-ies. Dent Mater. 2014 Apr;30(4):e41-78.
26. Çelık EU, Aladağ A, Türkün LŞ, Yilmaz G. Color changes of dental resin composites before and after polymerization and storage in water. J Esthet Restor Dent. 2011 Jun;23(3):179-88. 27. Setcos JC, Tarim B, Suzuki S. Surface finish produced on resin composites by new polishing systems. Quintessence Int. 1999 Mar;30(3):169-73.
Please cite this paper as: